Standard Test Method for Radial Crushing Strength, K, of Powder Metallurgy (P/M) Bearings and Structural Materials
The radial crushing strength test is a destructive procedure used to determine a material strength characteristic of PM bearings and hollow cylindrical test specimens. These data can be used to grade, classify, and evaluate the materials.
The PM bearing Specifications B438 and B439 require the use of this test method as an acceptance test for the strength of oil-impregnated sintered bearings.
This test method may be used by powder producers and parts manufacturers as a lot acceptance test for metal powders and lubricated powder mixtures intended for the production of porous parts.
Companies in the PM industry use this test as a manufacturing control test because it is appropriate for production practices.
Radial crushing strength is a property of the PM material but is not a design value. However, experience has shown that the radial crushing strength of a material is approximately twice the ultimate tensile strength.
1.1 This test method covers the equipment and laboratory procedure for the determination of the radial crushing strength of materials using either a plain powder metallurgy (PM) bearing or a thin-walled hollow cylindrical test specimen. This is a destructive test that produces quantitative results.
1.2.1 The principle of this procedure is based on the material being tested having minimal ductility. The permanent deflection of the cylinder during the test should not exceed 10 % of the outside diameter.
1.2.2 The radial crushing strength test results should be used only as a guide if the test specimen has a wall thickness that is greater than one-third of the outside diameter. These test results should then only be used for comparison with data from the test specimens of like materials and similar dimensions.
1.3 With the exception of density values, for which the g/cm3 unit is the industry standard, the values stated in inch-pound units are to be considered the standard. The values in SI units, shown in parenthesis have been converted in accordance with IEEE/ASTM Standard SI 10, may be approximate and are only included for information.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
Formato físico y digital
Nota: Precios sin IVA ni gastos de envío
Añadir a la cesta